Sandwich Structure Composite with Expandable Graphite Filled or Coated: Evaluation of Flame Retardancy and Mechanical Performances

Sandwich composites are increasingly used in high-performance application due to their high specific stiffness, strength and thermal insulation. The sandwich composites were developed using honeycomb and carbon fibre reinforced composite face sheet in this study. Expandable graphite (EG) weighting 5 wt% and 10 wt% were filled in honeycomb or coated on face sheet to improve the fireproof performance. The vertical burning test, cone calorimetry test, thermal insulation analysis, scanning electron microscopy and mechanical test were taken into account. With the increase of EG in the sandwich composites, a significant improvement on flame retardancy with better thermal insulation, lower values of peak heat release rate and MAHRE were confirmed for sandwich composite with EG both coated and filled. In addition, the sandwich with EG coated on face sheet presented better fire resistivity and thermal insulation properties when compared to that with EG filled in honeycomb. However, more total smoke release was also observed for EG coated composites due to partial combustion of resin within sufficient heat and oxygen. Furthermore, no significant effect on the mechanical properties of composites was confirmed from both fireproof approaches.


Introduction
Composite materials are one of the lightweight materials for transportation in-How to cite this paper: Zhu, C.K., Li, J.J., Ji, F.H., Yi, X.S., Rudd, C. and Liu, X.L. (2019) Sandwich Structure Composite with Expandable Graphite Filled or Coated: Evaluation of Flame Retardancy and Mechanical Performances. Open Journal of Safety Science and Technology, 9, 7-21. injury and death [6] [7]. Therefore, to use in structural applications, the fire resistance of the sandwich structures should be improved. In this case, the other available strategies developed is the application of flame retardants protection layer such as insulative materials or flame retardant coatings on heat-exposed surfaces of sandwich composite structures, or the application of flame retardant filler in the honeycomb or foam core to improve the thermal insulation performance.
Expandable graphite has been used in numerous applications of fire safety, especially thermal insulators and intumescent flame retardant for polymer composite [14] [15] [16]. Expandable graphite (EG) is equivalent to a staged version of a graphite-sulfuric acid salt; i.e. the graphene layers all remain intact while bisulfate ions are intercalated between these layers [17]. The key property of expandable graphite is the tendency to exfoliate when heated at high temperatures beyond a characteristic expansion onset temperature [18]. It expands rapidly in a worm-like manner to form vermicular graphite with a low density.
Kahlili et al. [19] who have worked on EG for polymer composite, and compared flame retardant properties of the composite with a surface coating and matrix filling, found that the composites both coated or filled with EG could provide a significant improvement on flame retardant performance.
However ing to investigate the effect of EG on the mechanical properties of sandwich, Therefore, the aim of this paper is to investigate the effect of EG on the flame retardant performance and thermal insulation properties of the sandwich composite. Two fireproof approaches, EG coated on the face sheet and EG filled in the core-honeycomb of sandwich, were taken into account in this study. The vertical burning test, cone calorimetry test and thermal insulation properties of the composite with both approaches were analysed for comparison.

Design and Manufacture of Sandwich Composites
The sandwich composites in this study were designed as Figure 1, which were produced from the carbon fibre/epoxy resin prepreg containing 49 wf% resin with an areal density of 345 g/m 2 (AVIC Composite, China). The Nomex honeycomb of an areal density of 240/m 2 was selected for core material (NHC-1, AVIC Composite, China). The manufacturing process was vacuum bagging at curing temperature. The skin with three layers prepreg was placed on the top and bottom of honeycomb, then covered by vacuum bag with vacuum at 1 bar and placed into the oven for 2 hours curing at 120˚C.
As can be seen from Table 1, there are five sample groups in this study. For flame retardant sandwich composites C-5 and C-10, the expandable graphite particles (180 μm mesh size and expansion ratio of 100:1) were sprayed on the face of skin and adhered by resin of prepreg before the vacuum bagging process, then vacuumed with 1 bar as well, and moved into the oven for curing at the same temperature. Additionally, the F-5 and F-10 composites where the expandable graphite was filled in the honeycomb with even distribution.

Vertical Bunsen Test
Vertical Bunsen testing was conducted to investigate the flame resistance of sandwich composites. Testing experiments were set up according to Federal Aviation Regulation (FAR) 25.853 standard of 60 s Vertical Bunsen burner testing specifications. The flame of methane gas was adjusted to the reach height of 38 mm flame above the top level of the burner barrel, which was 19 m below the edge of the specimen, and the flame was positioned under the centre of the specimen. There were three specimens for each group with a dimension of 305 mm (Length) × 75 mm (width) × 7.8 mm (thickness) individually hanged upright with the aid of a retort stand and clamp, and tested accordingly using burner (TESTech Instrument Technologies Co., Ltd, China). The burn length, drip flame time, flame time were studied and recorded.
Due to the sandwich structure and different materials on skin and core, the burning length of skin and core was both investigated, as such the cross-section of the sandwich composite was cut for measurement of the burn length of the sandwich structure.

Cone Calorimetry Test
The cone calorimeter tests were conducted on a cone calorimeter (Fire Testing Technology Ltd., UK) with sample dimension of 100 mm ×100 mm × nominal thickness and subjected to one-sided radiant heating according to the ISO5660-1 at the heat flow of 35 kW/m 2 . The heat exposed surfaces of the test specimens were placed 25 mm away from the cone heater. Cone calorimeter parameters including the time to ignition (TTI), time to flame out (TTFO), peak heat release rate (PHRR), total heat release (THR), total smoke release (TSR) and maximum average heat rate emission (MAHRE) were measured.

Thermal Insulation Property
The temperature on the fire retardant sandwich surface and the honeycomb were measured to estimate the thermal insulation performance. Two K-type thermocouples was attached on the surface of the sandwich specimen (T1) ex-C. K. Zhu et al. Open Journal of Safety Science and Technology posed to the flame and the opposite side surface (T3), respectively, and one was inserted into the honeycomb (T2) which had been marked in Figure 1. The surface of the sandwich was exposed to alcohol burner with a flame temperature of 500˚C for 1000 s, the time to thermal equilibrium temperature for each side and honeycomb was recorded.

Flexural Properties Analysis
To analyse the mechanical properties behaviour of the sandwich composite, the specimens were subjected to flexural test by three-point bending test through a 50KN UTM (MTS E42) following the ASTM C393. The specimens were prepared with 200 mm length, 75 mm width, and a span of 150 mm with the rate of loading was 2 mm/min.

Microstructure Observation
The micromorphology images of the char residues after cone calorimeter test were observed on a scanning electron microscope (SEM, Zeiss®, Germany) at a 10 KV voltage after sputtered with 5 nm gold using vacuum film deposition system (EM SCD500, Leica®, Germany).

Statistical Analysis
Statistical analysis was performed with GraphPad Prism (Version 7.00, Graph-Pad Software, San Diego, CA, USA) with unpaired t-tests. Confidence level was 95%.

Vertical Bunsen Burner Test
Vertical Bunsen Burner Test is a traditional method to investigate the flammability of materials. The results in Table 2 showed that the flammability of sandwich was reduced significantly with the incorporation of expandable graphite (EG) on the surface or into the honeycomb of the sandwich. The Flame Time of the sandwich was observed to decrease from 54 ± 5 s to 45 ± 2 s with the addition of EG into honeycomb from 0 wt% to 10 wt%. According to Figure 2 and Table 2, a decrease of Burn Length was also observed for sandwich composites with EG filling, and Burn Length of honeycomb was significantly lower than Skin for F-5 and F-10 sandwich composite respectively. This was attributed to the EG in the honeycomb rather than on the surface, the Skin-laminate with rich resin was ignited and burning with the fire whilst the EG was able to expand and form the worm-like char filling the gap of honeycomb, becoming the thermal barrier to prevent flame spreading along the Core.
With the same mass fraction of EG coated on the face sheet of sandwich composites, C-5 and C-10 presented lower Flame Time and Burn Length, when compared with EG filled sandwich (F-5 and F-10). The Flame Time was decreased to 30 ± 2 s and 6 ± 2 s for 5 wt% and 10 wt%, respectively. The first Open Journal of Safety Science and Technology  reason could be the EG on the face sheet of sandwich (Skin-Laminate) exposed to fire was fully expanded immediately, the formed thermal barrier on the composite surface could retard the flame spreading on the composite surface [19].

Cone Calorimetry Test
The effectiveness of fire-proofing approach filling the Expandable Graphite (EG) into the Honeycomb of sandwich or coat on the face sheet of the sandwich composite was evaluated. The HRR-time curve for sandwich composites were shown in Figure 3, and the detail data were recorded in Table 3. It was suggested that the fire reaction behaviour of the sandwich was significantly improved via filling the EG into a honeycomb of composite or coating EG on the face sheet.
Considering the first 100 s of thermal exposure, the reaction behaviour of composite with EG filled (F-5 and F-10) were similar to that of Control. The HRR of Control, F-5 and F-10 composites increased rapidly following self-sustained ignition, reaching the peak value of 322 ± 12, 293 ± 11, 260 ± 9 KW/m 2 , Open Journal of Safety Science and Technology  respectively. After 100 s, another HRR peaks were also observed at 197 s, 290 s and 334 s, with the peak values of 120 ± 6, 78 ± 5 and 61 ± 8 KW/m 2 , respectively. The behaviour of the second HRR peak was due to the burning of the back face sheet of sandwich composite. With the filling of EG from 0 wt% to 10 wt%, more char formed in the honeycomb to be the thermal barrier retard the fire and heat burning through the honeycomb and transfer into the back face sheet, as such 50% decrease of the second peak of HRR could be observed by 10 wt% EG filled (F-10) composite.
On the other hand, the HRR value of C-5 and C-10 composites with EG coated was found to increase slowly following ignition which was out in 100 s, resulting in lower PHRR value when compared to other composite groups (Control, F-5 and F-10). It was also attributed to the dense char layer formed from the expanded EG (Shown in Figure 4) provided a thermal-physical barrier Open Journal of Safety Science and Technology According to the data in Table 3 Figure 5. Normally, the EG exfoliation initialled when heated over 200˚C where the most of intercalating substances degraded and form gases escaped from the interlayer of EG resulting in expanding the graphite with a porous structure. As shown in Figure 5, the virgin EG received from the vendor was in the form of platelet with a diameter range of 210 -505 μm. After undergoing the thermal conditions caused by Cone Calorimetry Test, the EG expanded along the z-axis of EG and transformed to be vermicular structure, as such the similar diameter range to the virgin EG was observed for expanded graphite. Therefore, it was indicated that the EG filled in the honeycomb or coated on the face sheet could expand to form worm-like porous char and cross combine to be the dense char layer, which can prevent the fire and heat diffusion and reduce the heat release.

Thermal Insulation Test
In this paper, temperature-time profiles were collected at locations across the thickness of sandwich composites during the thermal insulation test. The temperature-time data at the front surface sheet of sandwich exposed to flame (T1), the honeycomb centre of sandwich (T2) and the back face sheet of the sandwich (T3) for all sandwich composites are shown in Figure 6. For T1 temperature of all composite, no significant difference was observed, while the T1 of steady-state (T1 SS ) was recorded at ⁓500˚C. However, referred to Figure 7, the C-5 and C-10 composite with EG coating cost ⁓400 s to reach the T1 SS , is much longer than that for Control, F-5 and F-10 composite. It was also attributed to the EG expanded on the surface of the face sheet exposed to fire; as such the heat conduction was retarded by the char layer, resulting in a delay of reaching steady thermal status.
For F-Composites with EG filling, the steady-status temperature of T2 (T2 SS ) was observed to decrease from ⁓500˚C (Control) to ⁓406˚C (F-5) and ⁓368˚C (F-10), due to the expanded EG in the honeycomb forming the thermal barrier region in the core of sandwich composite. Moreover, the T3 SS of F-Composite  with the addition of EG. Different from F-Composites, the fire-proof approach of C-Composites was using the EG on the face sheet to form dense char layer exposed to fire. Compared to Control, the T2 SS of C-Composite was decreased from ⁓500˚C to ⁓374˚C (C-5) and ⁓350˚C (C-10), respectively. In addition, the T3 SS of C-Composite was decreased from ⁓285˚C to ⁓239˚C (C-5), and ⁓235˚C (C-10). With the comparison between T1 and T3, the ∆T of all composite could be calculated to indicate the thermal insulation performance of sandwich with EG.
According to Figure 6 and Figure 7, with an increase of EG from 0 to 10 wt%, ∆T for F-Composite was increased from ⁓218˚C (Control) to ⁓227˚C (F-5) and ⁓254˚C (F-10), whilst that for C-Composite was increased to ⁓255˚C (C-5) and ⁓269˚C (C-10).
Therefore, the EG filled into the core-honeycomb and coated on the face sheet of the sandwich were available approaches to improve the flame retardancy and  considered during the application, so that the coordination with other flame retardant agent for EG coating could be a good approach to improve the fire retardant performance.

Mechanical Test
The effect of EG on the mechanical composite has been illustrated in literature, whilst the most of them were focused on the laminate composite with the EG mixed in the resin. As such, the effect of EG on the sandwich composite should be analysed and the mechanical performance of novel structure sandwich where the EG was filled in the honeycomb core or coated on the laminate skin could be compared. The Load-displacement curves of the specimens during the three-point bending test was shown in Figure 8. The sandwich structure with EG filled and coated had presented similar failure behaviour when compared to Control. As such, no significant difference was observed amongst the maximum load and the core shear failure of specimens with EG and Control. However, the sandwich with EG filled and coated was easier delaminated and failed with Open Journal of Safety Science and Technology core-to-face disband in the bending test. According to Figure 9, there is no significant difference figured out from the Core Shear Ultimate Strength ( ult s F ) and Face Stress around the sandwich structure with EG (F-5, F-10, C-5, C-10) and Control. This was confirmed that the sandwich structure was not influenced by the EG filled in the honeycomb or coated on the face sheet.

Conclusions
In this study, the sandwich composite was developed using carbon fibre reinforced composite and honeycomb. The expandable graphite (EG) was used to fill in the honeycomb of sandwich or coat on the face sheet of the sandwich to improve the fire-proofing performance.
According to the results, the burn length of the composite with the addition of EG in the vertical burning test was reduced significantly when compared to the control. With the addition of 10 wt% EG, the PHRR values were reduced from 322 to 103 KW/m 2 for C-Composite and 155 KW/m 2 for F-Composite. Additionally, the value of THR and MAHRE observed for F-Composite was reduced by 37% and 36%, whilst the decrease of C-Composite was 74% and 68%, respectively. However, the TSR value for F-Composite was observed to decrease by 43%, whilst that for C-Composite was increased by 35%. For thermal insulation performance of sandwich, C-Composite presented higher temperature difference between two face sheets than F-Composite with the same mass fraction of EG added. For mechanical properties analysis, no significant effect on the flexural properties could be figured out due to no influence on the interface and structure.
Therefore, the sandwich composite with EG coated or filled showed significant improvement on flame retardant performance and thermal insulation properties